Preparation of Scanning Tunneling Microscopy Tips Using Pulsed
Alternating Current EtchingLoyola eCommons Loyola eCommons
Faculty Publications and Other Works by Department
Preparation of Scanning Tunneling Microscopy Tips Using Pulsed
Preparation of Scanning Tunneling Microscopy Tips Using
Alternating Current Etching Alternating Current Etching
Victor A. Valencia
Avesh A. Thaker
Follow this and additional works at:
Part of the Chemistry Commons
Recommended Citation Recommended Citation Valencia, Victor A.;
Thaker, Avesh A.; Derouin, Johnathan; Valencia, Damian N.; Farber,
Rachael G.; Gebel, Dana A.; and Killelea, Daniel. Preparation of
Scanning Tunneling Microscopy Tips Using Pulsed Alternating Current
Etching. Journal of Vacuum Science and Technology A, 33, 2: 1-4,
2015. Retrieved from Loyola eCommons, Chemistry: Faculty
Publications and Other Works,
This Article is brought to you for free and open access by the
Faculty Publications and Other Works by Department at Loyola
eCommons. It has been accepted for inclusion in Chemistry: Faculty
Publications and Other Works by an authorized administrator of
Loyola eCommons. For more information, please contact
This work is licensed under a Creative Commons
Attribution-Noncommercial-No Derivative Works 3.0 License. ©
American Vacuum Society, 2015.
This article is available at Loyola eCommons:
Preparation of scanning tunneling microscopy tips using pulsed
alternating current etching
Victor A. Valencia, Avesh A. Thaker, Jonathan Derouin, Damian N.
Valencia, Rachael G. Farber, Dana A. Gebel, and Daniel R.
Killeleaa> Department of Chemistry and Biochemistry, Loyola
University Chicago, 1068 W. Sheridan Rd .. Chicago. Illinois
(Received 19 September 2014; accepted 3 December 2014; published 18
An electrochemical method using pulsed alternating current etching
(PACE) to produce atomically sharp scanning tunneling microscopy
(STM) tips is presented. An Arduino Uno microcontroller was used to
control the number and duration of the alternating current (AC)
pulses, allowing for ready optimization of the procedures for both
Pt:lr and W tips using a single apparatus. W tips prepared using
constant and pulsed AC power were compared. Tips fashioned using
PACE were sharper than those etched with continuous AC power alone.
Pt:lr tips were prepared with an initial coarse etching stage using
continuous AC power followed by fine etching using PACE. The number
and potential of the finishing AC pulses was varied and scanning
electron microscope imaging was used to compare the results.
Finally, tip quality using the optimized procedures was verified by
UHY-STM imaging. With PACE, at least 70% of the W tips and 80% of
the Pt:lr tips were of sufficiently high quality to obtain
atomically resolved images of HOPG or Ni(l 11 ). © 2014 American
Vacuum Society. [ http://dx.doi.org/10.1116/1.4904347 J
The scanning tunneling microscope (STM) has firmly established
itself as a powerful technique for surface charac terization and
analysis. 1 3 Central to the technique is the fact that the
resolution of the instrument is dependent on the sharpness of the
tip; in order to obtain images of surfaces with the component atoms
clearly discerned, an atomically sharp tip is rcquired.4 Reliable
fabrication of quality tips has been an issue since the development
of the STM,5 and over the past 30 years, many techniques have been
developed to provide reliable and robust tip preparation methods.
The techniques range widely, and often either require expensive,
specialized equipment for implementation or rely on seren dipity.
For example, in the initial report of imaging with STM, the tips
were formed by cutting a tungsten wire, then grinding the tip to a
point, and finally crashing into the sur face to "mini-spot weld"
the tip to a fine point.5 Other approaches include simple cutting,6
ion-milling of the
. 7 8 d I h . I h' 9- 14 Of . . tips, ' an c cctroc em1ca etc mg.
particular mtcrcst here is the electrochemical etching of tips;
electrochemical etching of W and Pt:lr wires is a promising method
for the reliable, economical, fabrication of high purity and
quality tips for STM. 15 18
The objective was to use an electrochemical technique to fashion
high quality tips with common, inexpensive equip ment. Of
particular note is the use of a commercially avail able,
inexpensive, microcontrollcr with a USB connection to
"Electronic mail: [email protected]
the computer and its packaged software. ln comparison, other
controlled tip etching techniques have employed DAQ computer boards
and custom software,9 or other specialized equipmcnt. 19·20 The
approach presented here is far less ex pensive and could be
implemented in almost any facility. Electrochemical etching is
attractive because it has been demonstrated to be effective in
fashioning tips for many
. 1 d 1 .. 1221 Frth . matcna s an app 1cat10ns. · u ermorc, a high
degree of tip purity can be realized by careful handling of the
etch ing solution and equipment. Several etching techniques have
been developed using both alternating current (AC) and direct
current (DC) power sources, 13·16 and while the details of the
process for AC and DC etching differ, both arc effec tive at
fashioning STM tips.21 ·22
Electrochemical etching yields highly tapered tips with an
extremely small radius of curvature ( < l µm) because the
etching rate of a wire dipped into an electrolytic solution is not
uniform across the bottom face of the wirc. 18·19 When the tip wire
was inserted into the solution, a meniscus forms , jutting up from
the liquid surface. When an electric potential is applied to the
tip wire, there is a concentration gradient of etchant ions within
the meniscus that results in a vortex of the etchant ions about the
tip apex as etching proceeds. The concentration of etchant ions is
lowest at the top of the me niscus (body of the tip wire) and
increases progressively to ward the base (tapered tip); as a
result , during the etching process, the etching rate is much
faster at the base of the wire than along the sides.9 For DC
etching, tip sharpness also depends on the ability to quickly shut
off the power to
023001-1 J. Vac. Sci. Technol. A 33(2), Mar/Apr 2015
0734-2101/2015/33(2)/023001/4/$30.00 © 2014 American Vacuum Society
023001 ·2 Valencia et al.: Preparation of STM tips using pulsed AC
the etching circuit at the moment the wire is etched to a point and
drops off, because further etching dulls the tip. To achieve this
aim, several techniques have been developed to quickly shut off the
DC voltage at the drop-off point.6•
Herein, an alternative approach is presented that utilizes pulses
of AC to drive the etching process. A key advantage is that the
eventual tip sharpness is not beholden to the abil ity to rapidly
stop the etching process because the microcon trollcr program
sends a set number of AC pulses. As a result, this technique
reliably fashions atomically sharp tips for STM. We detail a simple
apparatus that was used for the preparation of both Pt:lr and W
tips using the new, pulsed alternating current etching (PACE)
The PACE etching system used a variable AC power source (Variac) to
set the AC potential, a graphite counter electrode (1 cm diameter
graphite rod, McMaster-Carr), a custom made glass etching vessel
(Allen Scientific Glass), and an Arduino Uno microcontrollcr
(http://www.ardui no.cc) that controlled the number and duration
of AC pulses. The apparatus is depicted in Fig. l (a). The
glass-etching ves sel [Fig. 1 (b)J holds ~100 ml of etching
solution, having a diameter of 70 mm and a depth of 30 mm. The
vessel design was similar to the apparatus presented by Hagedorn et
and used a 15 mm diameter glass cylinder, with both the top and
bottom open, fused to the inner wall of the vessel. The cylinder
was IS mm deep, and the vessel was fi lled so the liquid level was
below the top of the small cylinder. The small glass cylinder
contained any surface disturbances caused by bubbling at the
graphite counter electrode. Therefore, etching occurred at a
well-defined, fixed depth beneath etching solution, yielding
high-quality tips. 15
The Arduino Uno microcontroller was connected to a simple
transistor and relay circuit, shown in Fig. 1 (c). One of the
digital I/0 pins (I/0 13) on the Arduino Uno was used to
FIG. 1. (Color Online) (a) Illustration of the electrochemical
etching station showing the electrodes and armngemenl of etching
solution reservoirs; (b) photograph of the glass etching container;
and (c) diagram of etching control circuit.
J . Vac. Sci. Technol. A, Vol. 33, No. 2, Mar/Apr 2015
Pio. 2. SEM image of a Pt:Ir tip after coarse etching stage showing
the bul bous tip remnant. Further fine etching removes the bulb
and fashions a sharp tip. Scale bar is 20 Jim.
activate a 2N2222 transistor. The transistor, in turn, con trolled
a relay (Quaz-SS-lOSD) that switched the current flow from the
Yariac. The Arduino Uno microcontroller pa rameters were set using
a packaged blinking LED control program (Arduino website), and
allowed the relay to deliver AC voltage pulses of 0.5 s duration
every 2s. The desired number of AC pulses was set in the software
for tip fabrica tion once the optimal number of AC pulses was
obtained from the optimization procedures detailed below. Pulse
dura tion and frequency, as well as the potential and frequency
(60 Hz) of the AC in the pulse, were measured during the etching
process with a digital oscilloscope with 1 MQ input impedance, and
the RMS AC potential was verified with a handheld multimeter. We
did not observe any undesired switching of the relay due to the
etching current load or any extraneous pulses from noise in the
circuit, and the pulse du ration was largely invariant for all of
the etches performed.
Ill. RESULTS AND DISCUSSION
A. Platinum:lridium Tips
Pt:lr tips were fashioned from 0.25 mm diameter Pt:Ir wire (80% Pt,
20% lr) (Advent Materials) using l .OM CaC)z (Aldrich, 99%) as the
etching solution. Etching of high quality Pt:lr tips required two
etching stages: an initial coarse stage using continuous AC power
followed by a fine stage using PACE. The two-stage process was
necessary because etching using PACE alone was time-consuming and
therefore undesirable. Alternatively, etching using only con
tinuous AC yielded tips with a bulbous deposit at the tip apex. A
scanning electron microscope (SEM) image of the bulbous tip of a
Pt:lr wire etched using only continuous AC is shown in Fig. 2. When
the two approaches were com bined, quality tips were reliably
fashioned . The coarse etch ing provided the gross shape, but left
the bulbous mass. After coarse etching, the PACE stage was used to
remove the bulb and prepared a tip suitable for STM imaging. A fur
ther benefit of using the two separate stages was that the overall
etching time was appreciably reduced because a higher potential
(faster etch rate) could be used for rough etching and the
low-voltage, slower etching rate was only needed for the final fine
The coarse etching stage was based on the Argonne Mcthod23 and
consisted of three different voltage steps. The
023001 ·3 Valencia et al. : Preparation of STM tips using pulsed AC
1 5 10 15 Number of Pulses
Fie. 3. SEM images of etched Pl:Ir tips after the fine etching
(PACE) stage for several conditions of pulse voltage and number of
pluses. The optimiza tion of the technique is apparent; tips
etching with a 1 V potential are not uniform, 5 V etching left a
blunt tip, whereas at 2.5 V, a sharp, uniform tip was observed
after five pulses. White scale bars are lOµm in all images.
tip was first etched for lOOs using a continuous AC potential of 35
V (RMS). The potential was then dropped to 30 V (RMS) for 50 s, and
finally, the tips were etched at 28 V until the tip was almost
entirely etched away and the bubbling ceased. Once coarse etching
was completed, the tip was inserted 2- 3 mm deeper into the
solution and the fine etching step was performed. As shown in Fig.
3, after the same coarse etching was performed, the optimal fine
etching PACE parameters were determined by varying the number and
voltage of the pulses, and their effects on the tip shape were
screened using SEM (Cambridge instruments S240) imaging. Figure 3
shows a grid of representative SEM images illustrating how the
optimal number of pulses and AC potential were determined. The
optimal parameters were five pulses at 2.5 V (RMS) AC; these
conditions consistently (>80%) yielded sharp, symmetric tips.
Etching above 2.5 Y, for example, 5.0 V (RMS), was able to rapidly
remove the bulb formation from the coarse stage. However, the tips
were persistently blunt, and did not achieve a similar degree of
sharpness after 15 pulses (or for fewer than five pulses, data not
shown), and further pulses had decreasing efficacy toward
sharpening. ln contrast, AC potentials below 2.5 V required more AC
pulses to remove the bulbous remnants from the initial coarse
stage, and once that was achieved, the tip quality rapidly
degraded, becoming spindly and deformed, as shown in the SEM images
for 1.0 V across the bottom of Fig. 3.
B. Tungsten Tips
The PACE method was able to etch high-quality tungsten tips as well
as Pt:lr. The W tips were fashioned from 0.25 mm diameter 99.95%
purity W wire (Advent Materials) using the setup shown in Fig. 1
(a). 4.0 M NaOH (Aldrich, 99%) solution (Nanopure water, 18 MQ cm)
was used as the etchant. As opposed to the two-step etching method
used for Pt:lr tips, the etching of high-quality W tips required
only a single stage. The W wire was inserted to a depth of
JVST A· Vacuum, Surfaces, and Films
Fie. 4. SEM images of W tips etched with constant 5 VAC ((a) and
(b)) and pulsed 2.5 VAC [(c) and (d)). The increased sharpness is
evident in (c) and (d) with the pulsed AC etching technique. Scale
bars are 2011m in all panels.
3 mm below the liquid surface, with the meniscus forming around the
wire. AC power was applied until bubbling from formation of H2
during the electrochemical etching of the tip ceased.24 The tip was
then extracted from the solution, rinsed with nanopurc water and
methanol, then dried in a stream of N2 gas. The etching solution
could be used for up to ten tips with little loss in performance.
However, after ten tips the etching time increased and the
likelihood of impur ities on the tip became more
The abilities of the PACE method arc highlighted by comparing the
sharpness of W tips etched with continuous AC to those etched with
the PACE method using SEM. Figure 4 shows images comparing tips
etched with both approaches, using the san1e etching solution. With
W, the bulbous formation at the apex formed on Pt:lr was not
observed. Panels (a) and (b) in Fig. 4 show W tips etched with
continuous AC power at a potential of 5 V (RMS); 5 V gave the
highest quality tips for continuous AC. Typical etching times using
continuous AC was around 90 s. As seen in the figure, the tip
geometry was symmetric, and a nice point was formed. ln comparison,
panels (c) and (d) of Fig. 4 show tips etched using PACE with a
potential of 2.5 V (RMS) AC. From Fig. 4 , it is apparent that the
PACE tips were even sharper than those fashioned using continuous
AC, and they retained the highly symmetric shape indicative of a
high-quality tip. For W tips, bulbous formations at the apex or
other irregularities were seldom observed with AC etching.
With the SEM screening of the tip quality completed, the
effectiveness of the PACE tip fabrication method was veri fied by
obtaining atomically resolved images in a UHV STM (RHK Technology,
Pan Scan with R9 controller). Both Wand Pt:lr tips were prepared
using PACE at a potential of 2.5 V (RMS) AC. The W tips were used
to image an HOPG surface, and Pt:lr tips were used to image both
HOPG and Ni(l 11) surfaces; all imaging was done under UHV (P <
l x 10- 9 Torr) conditions. The Pt:lr tips were used without any
additional treatment, but W tips were heat treated prior to
imaging. The STM chamber has a tip heating station where the tip is
brought to within a few millimeters
023001 -4 Valencia et al. : Preparation of STM tips using pulsed AC
FIG. 5. (Color online) STM images of HOPG using (a) etched W tips
(2 x 2nm, T= 80K, Vb=55 mV, /,=400pA); (b) Pt:Ir (5 x 5 nm, T= 80K,
Vb=50mV, l,=400pA); (c) STM image of Ni(l 11) using etched Pt:Tr
tip (10 x JO nm, T= 80K, Vb=20mV, 11 = 1.0nA). White scale bars are
1 nm for all images. The images are the unprocessed images obtained
with the UHV-STM system.
of a white-hot W filament. The heating was used to remove any
residual oxides on the W tips.25 As the tip was heated, the
pressure rose from the base pressure of 7 x 10- t 1 Torr into the
low 10- 9 Torr range, most likely a result of desorp tion from the
tip holder. Heating was continued for approxi mately l min after
the pressure in the chamber leveled off.
W tips etched using PACE were able to obtain atomically resolved
images 70% of the time on HOPG, out of a sample of ten tips. Figure
S(a) shows a representative, atomically resolved, STM image of HOPG
where a treated W tip was used. The yield for Pt: lr tips was even
greater; at least 80% of the tips fabricated (out of 40 tips) using
the pulsed AC technique gave atomic resolution on HOPG, a
representative STM image is shown in Fig. 5(b). Finally, the high
quality of the Pt:lr tips was further demonstrated by imaging a
Ni(l 11) surface, as shown in Fig. 5(c). The high yield of at least
80% for quality Pt:lr tips is in contrast to the typical 20% yield
for Pt:lr using the "cut-and-pull" technique in our lab (out of
more than 100 tips). Tips etched using either con tinuous AC or
suboptimal PACE parameters rarely yielded atomically resolved
images, and therefore, exact statistics of their efficacy were not
We have demonstrated that PACE is an inexpensive, straightforward
electrochemical etching technique that reli ably fashions tips for
STM imaging. Both W and Pt:lr tips were etched using the same
apparatus, and at least 80% of the Pt:lr tips (70% of W tips) were
capable of obtaining atomic resolution. Most notably, this system
J . Vac. Sci. Technol. A, Vol. 33, No. 2, Mar/Apr 2015
assembled with readily available equipment to etch either W and Pt:
lr tips by changing the etchant solution. The tip geo metries
after etching were screened with SEM imaging and the atomically
resolved STM images demonstrated the high quality of the tips. PACE
is clearly an economical, robust technique for the preparation of
This work was primarily supported by the College of Arts and
Sciences at Loyola University Chicago. Y. A. Valencia, J.
Derouin, D. A. Gebel, and A. A. Thaker thank Loyola Undergraduate
Research Opportunities (LUROP) for support through the Research
Mentoring Program, Provost Fellowships, and Mulcahy Scholars
Programs. Acknowledgment is made to the Donors of the American
Chemical Society Petroleum Research Fund for partial support of
this research through Grant PRF #54770-DNlS.
1D. M. Eigler, P. S. Weiss, E. K. Schweizer, and N. D. Lang, Phys.
Rev. Lett. 66, 1189 (1991).
2B. C. Stipe, M. A. Rezaei, and W. Ho, Science 280, 1732 (1998).
3J. Cerda, A. Michaelides, M. L. Bocquet, P. J. Feibelman, T.
Mitsui, M. Rose, E. Fomin, and M. Salmeron, Phys. Rev. Lett. 93,
4J. Tersoffand D.R. Hamann, Phys. Rev. B 31, 805 (1985). 5G.
Binnig, H. Rohrer, C. Gerber, and E. Weibel, Phys. Rev. Lett. 49,
6A. J. Melmed, J. Vac. Sci. Technol., B 9, 601 (1991). 7 M. J.
Va,ile, D. Grigg, J. E. Griffith, E. Fitzgemld, and P. E. Russell ,
J. Vac. Sci. Technol., B 9, 3569 (1991).
8S. W. Schmucker et al., Nat. Commun. 3, 935 (2012). "R. Stone, M.
Rosamond, K. Coleman, M. Peuy, 0. Kolosov, L. Bowen, V. Dubrovskii,
and D. Zeze, Rev. Sci. Tnstrum. 84, 035107 (2013).
10D. Gingery and P. Buehlmann, Rev. Sci. Tnstrum. 78, 11 3703
(2007). 11M. J. Zaccardi, K. Winkelmann, and J. A. Olson, J. Chem.
Educ. 87, 308
(2010). 12B. Ren, G. Picardi, and B. Pettinger, Rev. Sci. Tnstrum.
75, 837 (2004). 13M. M. Jobbins, A. F. Raigoza, and S. A. Kandel,
Rev. Sci. Tnstrum. 83,
036105 (2012). 14A. J. Nam, A. Teren, T. A. Lusby, and A. J.
Melmed, J. Vac. Sci.
Technol., B 13, 1556 (1995). 15T. Hagedorn, M. El Ouali, W. Paul,
D. Oliver, Y. Miyahara, and P.
Grueller, Rev. Sci. Tnstrum. 82, 113903 (2011). 16B.-F. Ju, Y.-L.
Chen, and Y. Ge, Rev. Sci. Jnstrum. 82, 013707 (2011). 17 A. W.
Liu, X. T. Hu, W. H. Liu, and G. J. Ji, Rev. Sci. Tnstrum. 68, 38
(1997). 18J. P. Tbe, P. P. Bey, S. L. Brandow, R. A. Brizzolara, N.
A. Burnham, D.
P. Dilella, K. P. Lee, C. R. K. Marrian, and R. J. Colton, J. Vac.
Sci. Technol., A 8, 3570 (1990).
1"w.-T. Chang, T.-S. Hwang, M.-T. Chang, C.-Y. Lin, W.-H. Hsu, and
J.-L. Hou, Rev. Sci. Tnstrum. 83, 083704 (2012).
2°R. Fainchtein and P.R. Zarriello, Ultramicroscopy 42, 1533
(1992). 21 G. J. Edwards and P. R. Pearce, J. Phys. D: Appl. Phys.
11, 761 (1978). 22S. L. Toh, H. Tan, J. C. Lam, L. C. Hsia, and Z.
H. Mai, J. Electrnchem.
Soc. 157, E6 (2010). 23STM Tip Fabrication and Characterization,
NST-SOP-122, Rev. 3,
Argonne National Labomtory. 24G. Tahmasebipour, Y. Ho.iiat, V.
Ahmadi, and A. Abdullah, Scanning 31,
65 (2009). 25Z . Q. Yu, C. M. Wang, Y. Du, S. Thevuthasan, and I.
Ultramicroscopy 108, 873 (2008).